Physicochem. Probl. Miner. Process. 52(1), 2016, 342−352 Physicochemical Problems of Mineral Processing www.minproc.pwr.wroc.pl/journal/ ISSN 1643-1049 (print) ISSN 2084-4735 (online) Received March 13, 2015; reviewed; accepted July 31, 2015 KINETIC GRINDING TEST APPROACH TO ESTIMATE THE BALL MILL WORK INDEX Hojjat H. GHAREHGHESHLAGH Hacettepe University Department of Mining Engineering, 06800 Beytepe Ankara, Turkey email@example.com Abstract: The standard Bond method is the most acceptable method for designing and selecting ball/rod mills described by their basic parameter called work index (Wi). The standard Bond method is a tedious time consuming procedure requiring at least 7 – 10 grinding cycles, so that many researchers have tried to simplify this method to be able to perform a rapid calculation of a work index. This study aims to develop a new approach toward estimating the Bond ball mill work index (BBWI) by applying a series of kinetic grinding tests with Bond standard mill. Establishing a series of relationships between grinding parameters and Bond equation parameters, this approach is fast and practical due to eliminating laboratory control steps while reducing the number of milling steps. In this scope, thirteen ore samples were used to compare Wi values obtained by standard Bond method with those of the proposed kinetic approach. The kinetic periods were determined as 0.33, 1, 2, 4 and 8 minutes. The results of kinetic tests were found to be logical and acceptable as they were so close to the values obtained by Bond standard method, for all samples error was ≤ 2.60%. It was therefore concluded that the proposed approach could be considered as a simple yet practical alternative for the standard Bond method. Keywords: work index, Bond method, kinetic grinding test, grindability, ball mill Introduction The standard Bond (1952; 1961) method is widely used in the course of design, selection, scale up, energy calculation and performance evaluation of grinding circuits in mineral processing industry. This is mainly owed to the wide and valid database this method uses to derive its empirical equation (Bond, 1952; 1960; 1961). The most important parameter in this empirical equation is the Bond work index (Wi) which expresses the resistance of a material to comminution. In mineral industry, this is generally used for comparing the resistance of different materials in milling, estimating the required energy for milling (Levin, 1989) and mill scaling-up (Man, 2002). http://dx.doi.org/10.5277/ppmp160129 Kinetic grinding test approach to estimate the ball mill work index 343 The Wi parameter is obtained from Bond’s ball mill grindability test (Bond, 1961). This test is performed according to the standard Bond procedure which proposed model is presented in Eq. 1. This standard grindability test simulates a closed-cycle dry grinding and screening process, which continues to carry out until the steady state condition of 250% circulating load is obtained. This grindability test is conducted in a Bond ball mill of ΦD/L= 0.3048/0.3048 m dimensions at the speed of 70 rpm. The mill is loaded with 21.125 kg standard sized balls and 700 cm3 of grinded materials to under 3.35 mm. The test procedure takes from 7 to 10 grinding cycles with the required amount of material for whole procedure being approximately 10 kg. Once steady state condition is achieved, the work index, Wi, can be calculated according to the following Eq. 1. 𝑊𝑖 = 48.95 𝐷 0.23 10 10 0.82 𝐺𝑏𝑝 ( − ) √𝑃80 √𝐹80 , 𝑘𝑊ℎ 𝑀𝑔 . (1) Determining Wi via the standard Bond method needs careful grinding cycles and screen procedures. However, these are tedious time-consuming procedures with potential errors in sieving steps. Considering the difficulties of the standard Bond method in the course of determining Wi, a number of simpler and faster alternative methods have been developed by various researchers (Berry and Bruce, 1966; Smith and Lee, 1968; Horst and Bassarear, 1977; Karra, 1981; Yap et al., 1982; Armstrong, 1986; Magdalinovic, 1989; Nematollahi, 1994; Aksani and Sonmez, 2000; Deniz and Ozdag, 2003; Yalcin et al., 2004; Ipek et al., 2005; Ahmadi and Shahsavari, 2009; Ahmadi et al., 2013). The aim of this study is to develop a new approach to estimate the Bond ball mill work index (BBWI) using a combination of Bond standard mill and initial test conditions by conducting kinetic grinding tests. The proposed approach differs from the previous methods in that it determines the required grinding parameters for calculating work index by the resultant distributions from the sieve analysis of the kinetic grinding tests, with no need to the control step using the 106 µm sieve. Although the same methodology was used for all materials, different relationships were established depending on the material. The kinetic method is implemented in two steps: 1) conducting laboratory grinding tests, and 2) calculation process in which the relationships between laboratory and Bond equation parameters are established. Method and material The experimental conditions of kinetic grinding tests together with mill specifications are given in Table 1. Except for grinding time, revolution numbers, sample amount and sieving procedures, all other operational conditions were set according to the standard Bond procedure. 344 H.H. Gharehgheshlagh Table 1. Conditions of kinetic grinding test and mill specifications (more in Appendix A) Dm,cm Lm, cm V, rpm Cv JB, % MB, kg dB, mm Geometry of mill liner Grinding type Vore, cm3 T, min 30.48 30.48 70 0.91 19.27 21.125 36.38 smooth dry 700 0.33, 1, 2, 4, 8 Thirteen samples of different ores and materials such as copper, iron and clinkers were collected for testing. According to the Bond method, these samples were prepared via repeated crushing in a laboratory jaw crusher following by sieving into appropriate sizes (100% < 3.35mm). Then, a representative feed sample of 700 cm3 was taken followed by measuring its weight (W). Particle size distribution of feed sample was measured, so that F80, F(-106) and Gfeed were determined. The proposed method The test procedure shown in Fig. 1 performs in the followings steps. Fig. 1. Kinetic grinding approach procedure for BBWI calculation Kinetic grinding test approach to estimate the ball mill work index 345 Kinetic grinding Exactly 700 cm3 of 100% passing 3.35 mm material from each sample was progressively grounded in periods of 0.33, 1, 2, 4, and 8 minutes. Our experience has shown that the required number of revolutions to achieve the circulating load of 250% is most likely to be between 200 to 300 rotations. However, it will be suitable to select a grinding time of 8 minutes (560 cycles) to ensure achieving the desired condition while creating an additional point to reduce the associated errors to the fitted model. After each grinding step, the mill contents were removed and dry sized. Particle size distributions were recorded for fresh feed as well as the product obtained at the end of each grinding step. As an example, particle size distributions of hematite sample are presented in Fig. 2. The Gtot(i), GNet(i) and P80(i) were determined graphically and numerically for each grinding step. Fig. 2. Kinetic grinding results, hematite sample t – NR conversion Referring to the mill speed, 70 rpm, the grinding period (t) was converted into the mill revolution number (NR). Relationship between NR and GNet In this step, a relationship was established between NR and GNet using non-linear least squares fitting techniques. The value of GNet was estimated for each NR using particle size distribution graphs obtained from the kinetic grinding tests in section 3.1, (NR(i), GNet(i)). An exponential relationship was found between NR and GNet with the corresponding equations presented in Table 3 for all samples. Figure 3 shows NR - GNet relation of hematite sample, as an example. 346 H.H. Gharehgheshlagh Table 3. Obtained NR - GNet equations for all samples Sample No. Ore type NR - GNet R2 1 Bauxite NR = 0.3883 GNet1.0624 0.9995 2 Hematite NR = 0.3749 GNet1.1178 1.0000 1.0984 0.9945 3 Chromite1 NR = 0.4171 GNet 4 Chromite2 NR = 0.4396 GNet1.0899 0.9998 1.0371 0.9985 5 Chalcopyrite1 NR = 0.5518 GNet 6 Chalcopyrite2 NR = 0.4673 GNet1.0489 0.9983 1.033 0.9982 7 Clinker1 NR = 0.6346 GNet 8 Clinker2 NR = 0.5097 GNet1.0574 0.9991 9 Dolomite NR = 0.5004 GNet 1.0486 0.9986 10 Magnetite NR = 0.3955 GNet1.0784 0.9995 1.032 0.9982 11 Limestone1 NR = 0.5937 GNet 12 Limestone2 NR = 0.7076 GNet0.9845 0.9989 13 Quartzite NR = 0.3523 GNet1.1083 0.9954 Fig. 3. NR - GNet relationships, hematite sample Relationship between NR and P80 Based on non-linear least squares fitting techniques, relationships among P80 values, P80(i), and NR values were established. These are polynomial relationships presented in Table 4 for all samples. Figure 4 shows the relationship between P80 and NR for the Hematite sample, as an example. In order to avoid extraneous oscillations in the cubic relationship established between NR and P80, a linear interpolation might be preferred. In Fig. 4, P80 increases with NR(280) possibly because of the agglomeration of fine particles. Kinetic grinding test approach to estimate the ball mill work index 347 Table 4. Obtained P80 – NR equations for all samples R2 Sample No. Ore type P80 – NR 1 Bauxite P80 = (–2E–06) NR3 + 0.0014 NR2 – 0.3094 NR + 87.923 0.968 2 Hematite P80 = (–1E–06) NR3 + 0.0011 NR2 – 0.2803 NR + 83.408 0.9971 3 Chromite1 P80 = (–2E–06) NR3 + 0.0017 NR2 – 0.3394 NR + 93.704 0.9647 4 Chromite2 P80 = (–9E–07) NR3 + 0.0008 NR2 – 0.1858 NR + 95.371 0.9876 3 2 5 Chalcopyrite1 P80 = (–2E–06) NR + 0.0015 NR – 0.3097 NR + 91.002 0.982 6 Chalcopyrite2 P80 = (–2E–06) NR3 + 0.0015 NR2 – 0.3464 NR + 102.7 0.9956 7 Clinker1 P80 = (–1E–06) NR3 + 0.0012 NR2 – 0.2643 NR + 95.144 0.9834 8 Clinker2 P80 = (–1E–06) NR3 + 0.0012 NR2 – 0.2426 NR + 92.183 0.9967 3 2 9 Dolomite P80 = (–1E–06) NR + 0.0011 NR – 0.2607 NR + 97.003 0.9831 10 Magnetite P80 = (–2E–06) NR3 + 0.0016 NR2 – 0.3955 NR + 102.23 0.9808 3 2 11 Limestone1 P80 = (–1E–06) NR + 0.0011 NR – 0.2605 NR + 94.201 0.9788 12 Limestone2 P80 = (–1E–06) NR3 + 0.0011 NR2 – 0.2836 NR + 104.38 0.9868 13 Quartzite P80 = (–1E–06) NR3 + 0.0009 NR2 – 0.1658 NR + 67.834 0.9566 Fig. 4. P80 - NR relationships, hematite sample Estimation of P80 and NR for 250% circulating load In the standard Bond grindability method, the CL of the grinding cycle is considered to be 250%. It means that the total charge in the mill is 350% or 3.5 times the fresh feed. Considering the weight W for all samples in the standard Bond grindability test, the purpose of the test will be to keep the passed amount of grinded material through the controlled sieve constant at W/3.5. Therefore, in order to reach the equilibrium 𝑊 grinding condition when CL is 250%, the GNet must be equal to 𝐺𝑁𝑒𝑡(250%) = (3.5) × 348 H.H. Gharehgheshlagh 100− 𝐹(−106) ( ). This is taken as the base-assumption-factor. The value of NR for 250% 100 CL, NR(250%), is determined by using GNet – NR plot or relationship, while the value of P80 for 250% CL, P80(250%), is determined by using NR – P80 plot or relationship. Estimation of Gbp(250%) The value of Gbp can be calculated by means of obtained NR and GNet values for 250% circulating load, Gbp(250%) = GNet(250%) / NR(250%). Calculation of BBWI (Wi) Finally, the BBWI or Wi can be calculated using the Bond equation (Eq. 1) and the estimated Gbp(250%) and P80(250%) parameters for kinetic grinding tests. Table 5. Comparison of standard Bond method and kinetic tests results Sample No. Ore type 1 Bauxite 2 Hematite 3 Chromite1 4 Chromite2 5 Chalcopyrite1 6 Chalcopyrite2 7 Clinker1 8 Clinker2 9 Dolomite 10 Magnetite 11 Limestone1 12 Limestone2 13 Quartzite Used Method P80 Gbp, g/rev Wi, kWh/t kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard kinetic test Bond Standard 66.42 65.21 63.48 62.97 81.30 81.09 83.83 81.56 74.44 75.11 78.03 78.62 87.78 85.24 86.74 87.02 82.45 80.56 71.31 73.25 79.66 79.48 86.16 87.22 62.40 64.39 1.771 1.779 1.374 1.365 1.358 1.384 1.360 1.349 1.460 1.457 1.601 1.592 1.304 1.260 1.410 1.398 1.505 1.510 1.598 1.579 1.400 1.398 1.548 1.551 1.527 1.555 10.321 10.172 12.525 12.531 14.330 14.082 14.649 14.497 13.054 13.150 12.298 12.416 15.471 15.625 14.865 14.999 13.479 13.249 11.806 12.120 13.998 13.997 13.646 13.727 11.238 11.282 Error, % -1.47066 0.04788 -1.76406 -1.04807 0.733376 0.951632 0.985496 0.898863 -1.73527 2.590589 -0.01085 0.584285 0.387378 Kinetic grinding test approach to estimate the ball mill work index 349 Comparison of the results of standard method and the kinetic tests Once the calculations were conducted, a comparison was performed between the results of the standard Bond method and those of kinetic tests and presented in Table 5. The complete Wi estimation procedure using the kinetic method is presented in Appendix A. Results and discussion In this study, a new approach was developed toward determination of the work index based on kinetic tests and Bond standard conditions. The GNet value for 250% CL was 100− 𝐹(−106) 𝑊 assumed as 𝐺𝑁𝑒𝑡(250%) = (3.5) × ( ). This assumption was taken as the 100 base-assumption-factor of the current study. The Bond method along with the kinetic approach was used to determine the work indices of different materials within thirteen samples. The results showed that the obtained values for work indices by means of kinetic tests were in good agreement with those of the standard Bond method, for all samples: error ≤ 2.60%, indicating usefulness of the Base-Assumption-Factor for estimation of Wi. The proposed procedure included five batch grinding tests, their sieve analyses in laboratory and the calculation process according to laboratory results and the Bond equation. This method is fast and practical as it eliminates laboratory control steps and reduces the number of milling steps. It also reduces the required weight of material from about 10 kg to approximately 1.5 kg. Due to these results and the simplicity of the method, the new developed approach can be used instead of the standard Bond method. It should be carefully noted that if an ore sample contains small amounts of very hard fractions, it will be necessary to apply a full Bond test to accumulate these fractions. This approach gives a raise to the possibility of using the collected data to change the test screen size and the assumed circulating load without collecting further data. This issue will be discussed in future studies. Acknowledgments The author gratefully acknowledges the financial support provided by the Turkish Scientific and Technical Research Council (TÜBİTAK) under grant No: B.02.1.TBT.0.06.01.00-215.01-847/6116 for 2215 program. Appendix A. Determination of the Bond work index using thekinetic method In order to determine Bond work index of a material, firstly, it must be prepared according to the Bond standard method. The kinetic method uses the same mill operating under the same conditions as those in Bond standard procedure, except for the grinding time, revolution numbers, sample amount and sieving procedure. Specifications of hematite sample, as an example, are presented in Table A.1. 350 H.H. Gharehgheshlagh Table A.1. Specifications of hematite sample 3 Vore,cm W, g F80, μm F(-106), % CL, % W/3.5, g 700 1022 1983 4.89 250 292.00 Calculation of Wi through the proposed kinetic method was performed at five grinding cycles. The sieve analysis of the fresh feed and these grinding cycles were measured and plotted. The obtained graph for the hematite sample is presented in Fig. 2, as an example. Then, the calculation procedure was conducted as follows: 𝑊 1. for a 250% circulating load, the net grinded material was 𝐺𝑁𝑒𝑡(250%) = ( ) × 3.5 100− 𝐹(−106) 2. 3. 4. 5. 6. 7. 8. ( ) = 279.27 g 100 each grinding period, t, was converted into a Mill Revolution Number, NR for each NR, the values of GNet and P80 were estimated through using particle size distribution graphs shown in Fig. 2 for hematite samples, an exponential relationship was established between NR and 1.1178 GNet (𝑁𝑅 = 0.3749 𝐺𝑁𝑒𝑡 , Fig. 3), so that 𝑁𝑅(250%) = 0.3749 × (279.27)1.1178 = 203.27 𝑟𝑒𝑣 for hematite sample, the following polynomial relationship was established between NR and P80: 𝑃80 = (−1𝐸 − 06)𝑁𝑅3 + 0.0011 𝑁𝑅2 − 0.2803𝑁𝑅 + 83.408 , Fig. 4, so that the P80 value for NR(250%) was calculated as 𝑃80(250%) = 63.48 𝜇𝑚 the grindability factor, Gbp, could be calculated by means of obtained NR and GNet for 250% circulating load: Gbp(250%)=(GNet(250%))/NR(250%) = 279.27/203.27 = 1.374 g/rev finally, the Bond equation was used to determine the work index, which was equal to 12.525 (kWh/Mg) in our example. Nomenclature BBWI Bond Ball Mill Work Index (kWh/Mg) CL Circulating Load (%) Cv Mill speed (fraction of critical) D Control sieve size = 106 μm dB Ball top size (mm) Dm Inner diameter of mill (cm) F(-106) Amount of -106 μm in the mil Feed, before grinding, (%) F80 80% passing size of the mill feed, before grinding, (μm) Gbp Grindibility factor (g/rev) Gbp(250%) Grindibility factor for 250% circulating Bond ball mill work index load (g/rev) Gfeed Weight of -106μm material in the mill feed, before grinding, (g) GNet Net grinding material of -106 μm (g) GNet(250%) Net grinding material under control sieve for 250% circulating load (g) Kinetic grinding test approach to estimate the ball mill work index 351 GNet(i) Weight of net grinding material of -106 μm for any step that is equal to Gtot(i) minus Gfeed for i=1,2,..,5 Gtot(i) Weight of -106 μm material in the mill product at any step (g) JB Ball load (% by volume) Lm Inner length of mill (cm) MB Total mass of balls (kg) NR Mill revolution numbers NR(250%) NR for 250% circulating load NR(i) amount of revolution number for each step, i = 1, 2, .., 5 P80 80% passing size of the final product (μm) P80(250%) P80 for 250% circulating load P80(i) 80% passing size of the -106μm material for any step for i=1,2,..,5 (μm) R 2 R-squared or coefficient of determination t Grinding period (min) V Mill speed (rpm) Vore Ore volume, required material (cm3) W Mass of mill content (g) W/3.5 Weight of material for 250% circulating load (g) Wi Work index (kWh/Mg) References AHMADI R., HASHEMZADEHFINI M., AMIRI PARIAN M., 2013, Rapid determination of Bond rodmill work index by modeling the grinding kinetics, Advanced Powder Technology 24, 441–445. AHMADI R., SHAHSAVARI SH., 2009, Procedure for determination of ball Bond work index in the commercial operations, Minerals Engineering 22, 104–106. AKSANI B., SONMEZ B., 2000, Simulation of Bond Grindability Test by Using Cumulative Based Kinetic Model, Minerals Engineering 13 (No. 6), 673-677. ARMSTRONG D.G., 1986, An alternative grindability test: an improvement of the Bond procedure, International Journal of Mineral Processing 16, 197–208. BERRY T.F., BRUCE R.W., 1966, A simple method of determining the grindability of ores, Can. Min. J. 87, 63–65. BOND F.C., 1952, The Third Theory of Comminution, Transaction AIME (Mining) 193, 484-494. BOND F.C., 1960, Three Principles of Comminution, Mining Congress Journal (August), 53-56. BOND F.C., 1961, Crushing and Grinding Calculation, British Chemical Engineering 6 (June & Aug.), 378-385 & 543-548. DENIZ V., OZDAG H., 2003, A new approach to Bond grindability and work index: dynamic elastic parameters, Minerals Engineering 16 (3), 211– 217. HORST W.E., BASSAREAR J.H., 1977, Use of simplified ore grindability technique to evaluate plant performance, Trans. Soc. Min. Eng. (AIME) 260, 348–351. IPEK H., UCBAS Y., HOSTEN C., 2005, The bond work index of mixture of ceramic raw materials, Mineral Engineering 18, 981-983. KARRA V.K., 1981, Simulation of Bond grindability tests, CIM Bull. 74, 195–199. 352 H.H. Gharehgheshlagh LEVIN J., 1989, Observation on the Bond Standard Grindability Test and a Proposal for a Standard Grindability Test for Fine Materials, Journal of South African Institute of Mining and Metallurgy 1, 13-21. MAGDALINOVIC N., 1989, A procedure for rapid determination of the Bond work index, International Journal of Mineral Processing 27 (1-2), 125–132. MAN Y.T., 2002, Why is the Bond Ball Mill Grindability Test done the way it is done?, European journal of mineral processing and environmental protection 2, 34-39. NEMATOLLAHI H., 1994, New size laboratory ball mill for Bond work index determination, Minerals Engineering, 352–353. SMITH R.W., LEE K.H., 1968, A comparison of data from Bond type simulated closed-circuit and batch type grindability tests, Trans. Soc. Min. Eng. (AIME) 24, 91–99. YALCIN T., IDUSUYI E., JOHNSON R., STURGESS C., 2004, A simulation study of sulphur grindability in a batch ball mill, Powder Technology 146 (Issue 3), 193-199. YAP R.F., SEPULVEDA J.L., JAUREGUI R., 1982, Determination of the Bond work index using an ordinary laboratory batch ball mill: Designing and Installation of comminution circuits, Soc. Min. Eng. (AIME), 176–203.